- Email: [email protected]

Journal of Magnetism and Magnetic Materials 290–291 (2005) 966–969 www.elsevier.com/locate/jmmm

Exchange constants and spin dynamics in Mn12-acetate A. Honeckera,, N. Fukushimaa,1, B. Normandb, G. Chaboussantc, H.-U. Gu¨deld a

Institut fu¨r Theoretische Physik, Technische Universita¨t Braunschweig, Mendelssohnstr. 3, 38106 Braunschweig, Germany b De´partement de Physique, Universite´ de Fribourg, 1700 Fribourg, Switzerland c Laboratoire Le´on Brillouin, CEA-Saclay, 91191 Gif-sur-Yvette Cedex, France d Departement fu¨r Chemie und Biochemie, Universita¨t Bern, Freiestrasse 3, 3000 Bern 9, Switzerland Available online 10 December 2004

Abstract We have obtained new inelastic neutron scattering (INS) data for the molecular magnet Mn12 -acetate which exhibit at least six magnetic peaks in the energy range 5–35 meV. These are compared with a microscopic Heisenberg model for the 12 quantum spins localised on the Mn ions, coupled by four inequivalent magnetic exchange constants. A ﬁt to the magnetic susceptibility under the constraint that the spin of the ground state be S ¼ 10 yields two dominant exchange constants of very similar value, J 1 J 2 65 K ( 5:5 meV), and two smaller exchange constants J 3 and J 4 : We compute the low-lying excitations by exact numerical diagonalisation and demonstrate that the parameters determined from the ground state and susceptibility ﬁt provide qualitative agreement with the excitations observed by INS. r 2004 Elsevier B.V. All rights reserved. PACS: 75.30.Et; 75.50.Xx; 78.70.Nx Keywords: Magnetic molecular materials; Heisenberg model; Susceptibility—magnetic; Neutron scattering—inelastic

Magnetic molecules present a fascinating new class of materials with a wide variety of applications (for a recent review see Ref. [1]). Coherent quantum phenomena in these mesoscopic systems are one focus of recent research [2]. Despite being among the ﬁrst generation of molecular magnets to be synthesised, Mn12 -acetate [3] remains that with the largest barrier to thermally activated tunnelling. Although much work has been devoted to Mn12 -acetate over the past decade, the microscopic mechanisms for the observed low-energy phenomena have remained controversial.

Corresponding author. Tel.: +49 531 391 5190; fax: +49 531 391 5833. E-mail address: [email protected] (A. Honecker). 1 Present address. University of the Saarland, Theoretische Physik, Geb. 38, 66123 Saarbru¨cken, Germany.

Here we discuss a microscopic exchange model for Mn12 -acetate. Twelve quantum spins Si are coupled by Heisenberg exchange interactions H¼

X

J ij Si Sj

(1)

i;j

with four different exchange constants J 1 ; J 2 ; J 3 and J 4 ; as represented in Fig. 1. Many experimental studies, including inelastic neutron scattering (INS) [4], show that the ground state (GS) of Mn12 -acetate has total spin S ¼ 10: This may be rationalised by considering an arrangement of eight parallel spins S ¼ 2 on the crown Mn3þ ions oriented antiparallel to four aligned S ¼ 32 spins on the core Mn4þ ions (Fig. 1). The S ¼ 10 GS imposes a strong constraint on the allowed exchange constants in Eq. (1), excluding [5,6] a number of parameter sets proposed

0304-8853/$ - see front matter r 2004 Elsevier B.V. All rights reserved. doi:10.1016/j.jmmm.2004.11.302

ARTICLE IN PRESS A. Honecker et al. / Journal of Magnetism and Magnetic Materials 290–291 (2005) 966–969 J4

J4 J2

J2 J3

J1

Fig. 1. Magnetic exchange model for Mn12 -acetate. Arrows denote the twelve Mn ions: eight Mn3þ ions on the crown have local spin S ¼ 2 while four Mn4þ ions in the core have S ¼ 32: Lines show exchange paths with interaction parameters J 1 ; J 2 ; J 3 and J 4 :

60

parameter set A parameter set B parameter set C parameter set D parameter set E

Tχ [emu K/mol]

50

40

30

20

10

0 0

50

100

150

200

250

300

T [K] Fig. 2. Static magnetic susceptibility. Filled and open circles are measured respectively on a deutered sample under a ﬁeld of 0.1 T [6] and on a non-deuterated sample at 1 T [8]. Lines are obtained from an 8th-order high-temperature series for the parameter sets in Table 1.

in the literature, such as that obtained by the ab initio local density approximation [7]. The magnetic susceptibility w is a valuable quantity in the determination of magnetic exchange constants. Fig. 2 shows two results for w; measured with an ordinary sample under an applied ﬁeld of 1 T [8], and with a deuterated sample at 0.1 T [6]. Both data sets agree well for temperatures between 40 and 300 K despite the different conditions, demonstrating the reliability of the susceptibility measurement at high temperatures. Exchange constants can then be determined by comparison with a symbolic high-temperature series expansion. In

967

combination with a numerical test of the S ¼ 10 groundstate requirement, this restricts the possible parameters to a narrow region around J 1 J 2 60 K, J 3 J 4 ¼ 5–10 K [6]. Columns A, B and C of Table 1 list three choices of parameters in this region (parameter set A was used in [6]). Columns D and E contain the parameter sets proposed in Refs. [9,10] respectively. The lines in Fig. 2 show the susceptibility w obtained from an average of four different Pade´ approximants to the eighth-order high-temperature series [6] evaluated with the corresponding parameters. The last row of Table 1 lists the effective g-factor entering the absolute value of w (electron paramagnetic resonance [11] yields geff ¼ 1:968). Parameter sets A, B and C yield good agreement with the experimental results, whereas the results for sets D and E are in clear disagreement. We conclude that the exchange constants proposed in Refs. [9,10] are incompatible with w: A number of magnetic excitations in the range of 5–35 meV has been observed by INS experiments performed on different spectrometers [12,6]. The points in Fig. 3 show the spectrum obtained on the MARI spectrometer at ISIS with an incident energy E i ¼ 17 meV. Five magnetic excitations can be identiﬁed unambiguously in this data, and are shown by the lines in Fig. 3, which are ﬁts with Gaussian curves on a linear background. Analysis of their Q- and T-dependence identiﬁes these ﬁve excitations as magnetic and at least the lowest two of spin S ¼ 9 [6]. A further magnetic excitation at 27 meV is the ﬁrst candidate for an S ¼ 11 excitation [6], in accordance with high-ﬁeld magnetisation measurements; this energy sets a lower bound for the numerical calculations. We have performed exact diagonalisation for the model Hamiltonian (1), both to verify the S ¼ 10 GS and to determine the low-lying excitations. The lowest excited states in the sectors with spin 8pSp11 are listed in Table 1 in ascending order of energy (for sets A, D and E these extend results presented in Refs. [6,9,10]). Spatial symmetry is described by a momentum k such that the wave function acquires a phase factor eik under a 90 rotation of the model in Fig. 1. The letters in Fig. 3 show the energies of the lowest S ¼ 9 excitations for the corresponding data sets in Table 1. A constant shift of 1:29 meV is added to all computed energies [6] to account for the uniaxial cluster anistropy. Parameter set D [9] provides only four instead of the observed ﬁve levels in the energy range of the ﬁgure. Although set E [10] yields qualitative agreement with the lowest S ¼ 9 excitations, it is not only inconsistent with w; but also fails to explain the magnetic excitations observed by INS around 30 meV [6]. Parameter sets A, B and C all provide qualitative agreement with the ﬁve S ¼ 9 excitations, and the lowest S ¼ 11 excitation, observed by INS. Set A yields the best

ARTICLE IN PRESS A. Honecker et al. / Journal of Magnetism and Magnetic Materials 290–291 (2005) 966–969

968

Table 1 Energy E and symmetry k of low-lying excitations for a Mn12 -acetate exchange model with different parameter sets (A) [6] J 1 ¼ 67:2; J 2 ¼ 61:8; J 3 ¼ 7:8; J 4 ¼ 5:6

(B) J 1 ¼ 64:5; J 2 ¼ 60:3; J 3 ¼ 4:2; J 4 ¼ 6:3

(C) J 1 ¼ 64; J 2 ¼ 65; J 3 ¼ 11; J 4 ¼ 4

(D) [9] J 1 ¼ 119; J 2 ¼ 118; J 3 ¼ 8; J 4 ¼ 23

(E) [10] J 1 ¼ 115; J 2 ¼ 84; J 3 ¼ 4; J 4 ¼ 17

E (K)

k

E (K)

k

E (K)

k

E (K)

k

E (K)

k

S¼8

56:52 59:49 61:07

p p 0

58:07 61:08 61:78

p p 0

57:13 60:18 62:37

p p 0

68:12 69:81 73:55

p 0 p

78:39 82:26 83:49

p 0 p

S¼9

28:48 44:47 91:46 119:67 159:61 304:45

p=2 p 0 p=2 p 0

29:15 40:71 81:82 113:42 154:43 297:02

p=2 p 0 p=2 p 0

28:92 48:22 102:96 132:51 175:62 308:05

p=2 p 0 p=2 p p

33:99 35:76 65:11 174:55 267:13 501:03

p=2 p 0 p=2 p 0

39:13 45:43 77:12 124:63 179:93 436:52

p=2 p 0 p=2 p 0

S ¼ 10 293:74 297:30

p=2 p

285:63 289:27

p=2 p

295:02 297:79

p=2 p

507:87 509:01

p p=2

435:95 436:83

p p=2

S ¼ 11 285:58 303:23

0 p=2

274:17 313:84

0 p=2

287:41 290:80

0 p=2

510:38 696:91

0 p=2

429:66 537:96

0 p=2

geff

1:935

1:935

1:92

2:12

2:1

Exchange constants are given in Kelvin (K). The GS has spin S ¼ 10 in all ﬁve cases. No energetic correction is applied for uniaxial anisotropy of the cluster.

Intensity [arb. units]

5

C

C

C

B B 4

A

B

A

C

C

B A

B A

A

3

2

1

D D

D

EE

D E

E

E

0 0

2

4

6

8

10

12

14

16

18

Energy transfer [meV] Fig. 3. Magnetic excitations. Points show the INS spectrum obtained on MARI with T ¼ 8 K, E i ¼ 17 meV and 1pQp2 A˚1 : Lines are Gaussian ﬁts on a linear background. Letters represent numerical results for the S ¼ 9 excitations listed in Table 1 for the corresponding parameter choices. A constant energy 1:29 meV has been added to all calculated energies to account for magnetic anisotropy effects [6].

quantitative agreement [6], while B and C yield an estimate of the error bars: although the individual J i values differ by no more than 3:2 K, the low-lying S ¼ 9

levels may shift by as much as 16 K (1.4 meV) from set A to set C. This demonstrates the high sensitivity of the excitation spectrum to small changes in the exchange constants. Transitions from the S ¼ 10 GS to states with Sp8 are not observable by INS due to selection rules. However, our results predict further low-lying excitations with So9: In particular, the S ¼ 8 excitations in Table 1 may be interpreted as scattering states of a pair of the lowest S ¼ 9 states (k ¼ p=2). In summary, we have determined the microscopic exchange parameters of Mn12 -acetate as J 1 J 2 65 K, and J 3 ; J 4 5–10 K. Earlier proposals [5,9,10] are inconsistent with the magnetic susceptibility, and do not match our new INS results. Further improvements to the optimal parameter set would require a treatment of the uniaxial anisotropies at the single-ion level, which would be expected to reduce the spread of the S ¼ 9 levels, thereby improving agreement with the INS data. This work was supported by the Swiss National Science Foundation, the TMR programme Molnanomag of the European Union (No: HPRN-CT-199900012), and by the Deutsche Forschungsgemeinschaft through Grant SU 229/6-1.

ARTICLE IN PRESS A. Honecker et al. / Journal of Magnetism and Magnetic Materials 290–291 (2005) 966–969

References [1] J. Schnack, Lect. Notes Phys. 645 (2004) 155. [2] I. Tupitsyn, B. Barbara, in: J.S. Miller, M. Drillon (Eds.), Magnetism: Molecules to Materials III, Wiley-VCH, Weinheim, 2002. [3] R. Sessoli, et al., J. Amer. Chem. Soc. 115 (1993) 1804. [4] I. Mirebeau, et al., Phys. Rev. Lett. 83 (1999) 628.

[5] [6] [7] [8] [9] [10] [11] [12]

969

C. Raghu, et al., Phys. Rev. B 64 (2001) 064419. G. Chaboussant, et al., Phys. Rev. B 70 (2004) 104422. D.W. Boukhvalov, et al., Phys. Rev. B 65 (2002) 184435. A.R. Schake, et al., Inorg. Chem. 33 (1994) 6020. N. Regnault, et al., Phys. Rev. B 66 (2002) 054409. K. Park, et al., Phys. Rev. B 69 (2004) 014416. A.L. Barra, et al., Phys. Rev. B 56 (1997) 8192. M. Hennion, et al., Phys. Rev. B 56 (1997) 8819.

Copyright © 2020 COEK.INFO. All rights reserved.